# Assessment of the Effect of Residual Stresses Arising in the HAZ of Welds on the Fatigue Life of S700MC Steel

^{*}

## Abstract

**:**

## 1. Introduction

^{−1}. The reason for the reduction of the heat input value is the intense grain coarsening in the HAZ and, for higher-strength steels, the softening of the structure, which can occur at the interface between the HAZ and the base material. Many studies have investigated grain coarsening and its effect on mechanical properties. For example, Bayock et al. [13] investigated the effect of heat input on the microstructure and mechanical properties of dissimilar S700MC/S960QC steels. Three different heat input values (15, 7 and 10 kJ·cm

^{−1}) were used. The best microstructure formation was obtained using a heat input of 10 kJ·cm

^{−1}. The S700MC steel was investigated by Górka [14] and also by Moravec et al. [15]. The aim of these studies was to determine the properties and microstructure of the HAZ of S700MC steel. The steel with higher strength properties was investigated by Mičian et al. [16]. In the study, the effect of the cooling rate on the mechanical properties of the heat-affected zone of the steel S960MC was investigated. Furthermore, Jambor et al. [17] dealt with the development of the microstructure in the HAZ of the S960MC steel GMAW weld.

## 2. Materials and Methods

_{g}and A

_{80}were measured at room temperature—RT. The testing device TIRA Test 2300 (TIRA GmbH, Schalkau, Germany) was used. Static tensile test was performed according to standard EN ISO 6892-1 with loading rate 1 mm/min up to achieving YS and after that 15 mm/min. The mechanical properties of the annealed material at 550 °C were measured. The reason for the annealing was to eliminate the surface residual stresses in the sample that were created during the machining process. The annealing of the samples was carried out in a Reetz vacuum furnace (HTM Reetz GmbH, Berlin, Germany). The heating rate was the same for all experiments and was stepwise (0.8 °C·min

^{−1}to 80 °C; 1.5 °C·min

^{−1}to 220 °C; 2 °C·min

^{−1}to 300 °C and 4 °C·min

^{−1}in the temperature range 300 to 550 °C). The holding time at the annealing temperature was 2 h. Additionally, the cooling rate of the sample was the same for all experiments and in this case was constant (5 °C·min

^{−1}). The heat treatment was carried out under vacuum, which was 7 × 10

^{−5}mbar. The determination of the residual stresses by XRD method confirmed that only minimal residual stresses were present in the annealed samples (550 °C for 2 h). Table 2 shows the average values of the mechanical properties of the base and annealed material obtained from 5 measurements.

^{−1}. The temperature cycles in the HAZ of the welds were measured by the thermocouples type R, connected to a DiagWeld apparatus (Technical University of Liberec, Liberec, Czech Republic) with a recording frequency of 50 Hz.

_{1}= −1.25 TPa

^{−1}and ½𝑠

_{2}= 5.75 TPa

^{−1}were used to convert deformation to stress. The value of the diffraction angle of the {211} α–Fe planes of the material in the undeformed state is 156° 2θ. These values were used from the XDR Win2000 software database. The diffraction angles were determined by the Gaussian function approximation using the Absolute Peak method. The algorithm for calculating the residual stresses was sin

^{2}ψ.

## 3. Experiments and Results

- (1)
- Obtaining a real temperature cycle corresponding to MAG welding with heat input up to 10 kJ·cm
^{−1}; - (2)
- Experimental setting of the annealing conditions (T = 550 °C; t = 2 h) at which the surface residual stresses created during the machining of the test samples are reduced;
- (3)
- Determination of mechanical properties and S–N curves for the base and annealed materials;
- (4)
- Application of a temperature–stress cycle to annealed samples (produced in accordance with Figure 2) in a Gleeble 3500;
- (5)
- Determination of the residual stresses in the samples using the XRD method;
- (6)
- Annealing to reduce residual stresses after application of temperature–stress cycle in device Gleeble 3500 realized for some samples;
- (7)
- Determination of S–N curves for the state corresponding to the influence of the temperature–stress cycle (with residual stresses) and also for the state after application of the temperature–stress cycle but with subsequent annealing to reduce residual stresses.

#### 3.1. Measurement and Application of Temperature Cycles

#### 3.2. Analysis of Residual Stresses after Machining and after Annealing

#### 3.3. Determination of S–N Curve for Base Material S700MC and Annealed Material

^{7}cycles. A total of 10 samples were tested for each variation—one sample for each stress level. The base material was tested at stress levels of 580; 550; 527.5; 505; 490; 475; 468; 461; 455 and 447.5 MPa and for the annealed material, stress levels of 580; 565; 550; 546; 542.5; 535; 527.5; 520; 500 MPa were chosen. The measured S–N curves of the base and annealed material are shown in Figure 6. The achieved fatigue life of the base material was σc = 447.5 MPa and the achieved fatigue life of the heat-treated material was σc = 500 MPa. Table 3 shows the fatigue test results for the base and annealed materials.

#### 3.4. Application of Temperature Cycles in the Gleeble 3500

^{−3}Torr in a controlled deformation mode. A rigid clamping of the sample was defined with zero dilation monitored by the L-Gauge contact strain gauge. This procedure was repeated for all 20 test samples so that the distribution and magnitude of residual stresses were the same in all samples.

_{1}= 13.24 µm, d

_{2}= 13.09 µm and d

_{3}= 13.28 µm were obtained. The average mean grain size in the highly heated area is d

_{s}= 13.21 µm.

#### 3.5. Analysis of Residual Stresses after Application of the Temperature–Stress Cycle

#### 3.6. Fatigue Life Determination of Samples with Residual Stresses

^{7}cycles. The samples were loaded at stress levels of 520; 490; 460; 400; 370; 360; 350; 345; 340 and 335 MPa. Again, a total of 10 samples were tested, one for each stress level. The fatigue test results for the samples with residual stresses are shown in Table 4 and the S–N curve is shown in Figure 11.

## 4. Discussion

_{c}are basic and important material characteristics for dynamically loaded parts. The use of HSLA steels in automotive applications requires information about the fatigue life of these steels. It is easier to obtain S–N curves of base materials than to obtain S–N curves of materials affected by a technological process such as welding.

_{c}of 10%, from 447.5 MPa to 500 MPa. EBSD analysis confirmed that there was no increase in the mean grain size.

_{c}was decreased to 335 MPa, i.e., by 33% compared to the annealed material.

## 5. Conclusions

- (1)
- After annealing the S700MC steel samples (550 °C_2 h), the YS value remained unchanged but the UTS value decreased by 7.8%. At the same time, the fatigue strength increased by 10%, from 447.5 MPa to 500 Mpa;
- (2)
- Application of the temperature–stress cycle caused residual tensile stresses in the sample with a maximum value of 507 MPa and compressive residual stresses with a maximum value of 471 Mpa;
- (3)
- The application of the temperature–stress cycle also caused a decrease in the fatigue strength σ
_{c}from 500 MPa to 335 MPa, i.e., a decrease of 33%; - (4)
- Annealing at 550 °C for 2 h caused the complete elimination of compressive residual stresses and a significant 80% reduction in tensile residual stresses in the samples subjected to the temperature–stress cycle. As a result, the fatigue strength of the samples increased from 335 MPa to 450 Mpa;
- (5)
- According to the above, residual stresses contribute to 69% of the fatigue strength reduction. The residue is due to material changes;
- (6)
- The samples with residual stresses fractured at a point 3.7 mm from the center of the sample, thus up to the tensile stress peaks. This is probably related to the redistribution of residual stresses that occur during cyclic loading.

## Author Contributions

## Funding

## Data Availability Statement

## Conflicts of Interest

## References

- De Meester, B. The Weldability of Modern Structural TMCP Steels. ISIJ Int.
**1997**, 37, 537–551. [Google Scholar] [CrossRef] - Ufuah, E.; Ikhayere, J. Elevated Temperature Mechanical Properties of Butt-Welded Connections Made with High Strength Steel Grades S355 and S460M. In Design, Fabrication and Economy of Metal Structures; Springer: Berlin/Heidelberg, Germany, 2013; pp. 407–412. [Google Scholar]
- Lee, C.-H.; Shin, H.-S.; Park, K.-T. Evaluation of High Strength TMCP Steel Weld for Use in Cold Regions. J. Constr. Steel Res.
**2012**, 74, 134–139. [Google Scholar] [CrossRef] - Zavdoveev, A.; Poznyakov, V.; Baudin, T.; Rogante, M.; Kim, H.S.; Heaton, M.; Demchenko, Y.; Zhukov, V.; Skoryk, M. Effect of Heat Treatment on the Mechanical Properties and Microstructure of HSLA Steels Processed by Various Technologies. Mater. Today Commun.
**2021**, 28, 102598. [Google Scholar] [CrossRef] - Illescas Fernandez, S.; Fernández, J.; Asensio, J.; Sánchez Soto, M.; Guilemany Casadamon, J.M. Study of the Mechanical Properties of Low Carbon Content HSLA Steels. Rev. Metal.
**2009**, 45, 424–431. [Google Scholar] [CrossRef][Green Version] - Fernández, J.; Illescas, S.; Guilemany, J. Effect of Microalloying Elements on the Austenitic Grain Growth in a Low Carbon HSLA Steel. Mater. Lett.
**2007**, 61, 2389–2392. [Google Scholar] [CrossRef] - Barbaro, F.; Kuzmikova, L.; Zhu, Z.; Li, H. Weld HAZ Properties in Modern High Strength Niobium Pipeline Steels. In Energy Materials 2014; Springer: Berlin/Heidelberg, Germany, 2014; pp. 657–664. [Google Scholar]
- Nazarov, A.; Yakushev, E.; Shabalov, I.; Morozov, Y.D.; Kireeva, T. Comparison of Weldability of High-Strength Pipe Steels Microalloyed with Niobium, Niobium and Vanadium. Metallurgist
**2014**, 57, 911–917. [Google Scholar] [CrossRef] - Schaupp, T.; Schroepfer, D.; Kromm, A.; Kannengiesser, T. Welding Residual Stresses in 960 MPa Grade QT and TMCP High-Strength Steels. J. Manuf. Process.
**2017**, 27, 226–232. [Google Scholar] [CrossRef] - Laitila, J.; Larkiola, J. Effect of Enhanced Cooling on Mechanical Properties of a Multipass Welded Martensitic Steel. Weld. World
**2019**, 63, 637–646. [Google Scholar] [CrossRef][Green Version] - Branco, R.; Berto, F. Mechanical Behavior of High-Strength, Low-Alloy Steels. Metals
**2018**, 8, 610. [Google Scholar] [CrossRef][Green Version] - Taavitsainen, J.; da Silva, P.S.V.; Porter, D.; Suikkanen, P. Weldability of Direct-Quenched Steel with a Yield Stress of 960 MPa. In Proceedings of the 10th International Conference on Trends in Welding Research and 9th International Welding Symposium of Japan Welding Society (9WS), Tokyo, Japan, 11–14 October 2016; Curran Associates, Inc.: Red Hook, NY, USA, 2017; pp. 11–14. [Google Scholar]
- Njock Bayock, F.; Kah, P.; Mvola, B.; Layus, P. Effect of Heat Input and Undermatched Filler Wire on the Microstructure and Mechanical Properties of Dissimilar S700MC/S960QC High-Strength Steels. Metals
**2019**, 9, 883. [Google Scholar] [CrossRef] - Górka, J. Microstructure and Properties of the High-Temperature (HAZ) of Thermo-Mechanically Treated S700MC High-Yield-Strength Steel. Mater. Tehnol.
**2016**, 50, 617–621. [Google Scholar] [CrossRef] - Moravec, J.; Novakova, I.; Sobotka, J.; Neumann, H. Determination of Grain Growth Kinetics and Assessment of Welding Effect on Properties of S700MC Steel in the HAZ of Welded Joints. Metals
**2019**, 9, 707. [Google Scholar] [CrossRef][Green Version] - Mičian, M.; Harmaniak, D.; Nový, F.; Winczek, J.; Moravec, J.; Trško, L. Effect of the T8/5 Cooling Time on the Properties of S960MC Steel in the HAZ of Welded Joints Evaluated by Thermal Physical Simulation. Metals
**2020**, 10, 229. [Google Scholar] [CrossRef][Green Version] - Jambor, M.; Ulewicz, R.; Nový, F.; Bokůvka, O.; Trško, L.; Mičian, M.; Harmaniak, D. Evolution of Microstructure in the Heat Affected Zone of S960MC GMAW Weld. Mater. Res. Proc.
**2018**, 5, 78–83. [Google Scholar] - Kik, T. Computational Techniques in Numerical Simulations of Arc and Laser Welding Processes. Materials
**2020**, 13, 608. [Google Scholar] [CrossRef][Green Version] - Kik, T. Heat Source Models in Numerical Simulations of Laser Welding. Materials
**2020**, 13, 2653. [Google Scholar] [CrossRef] - Nassiraei, H.; Rezadoost, P. Stress Concentration Factors in Tubular X-Connections Retrofitted with FRP under Compressive Load. Ocean Eng.
**2021**, 229, 108562. [Google Scholar] [CrossRef] - Nassiraei, H.; Rezadoost, P. Stress Concentration Factors in Tubular T/Y-Connections Reinforced with FRP under in-Plane Bending Load. Mar. Struct.
**2021**, 76, 102871. [Google Scholar] [CrossRef] - Nassiraei, H.; Rezadoost, P. SCFs in Tubular X-Connections Retrofitted with FRP under in-Plane Bending Load. Compos. Struct.
**2021**, 274, 114314. [Google Scholar] [CrossRef] - Nassiraei, H.; Rezadoost, P. Parametric Study and Formula for SCFs of FRP-Strengthened CHS T/Y-Joints under out-of-Plane Bending Load. Ocean Eng.
**2021**, 221, 108313. [Google Scholar] [CrossRef] - Lahtinen, T.; Vilaça, P.; Infante, V. Fatigue Behavior of MAG Welds of Thermo-Mechanically Processed 700MC Ultra High Strength Steel. Int. J. Fatigue
**2019**, 126, 62–71. [Google Scholar] [CrossRef] - Kim, Y.; Hwang, W. Effect of Weld Seam Orientation and Welding Process on Fatigue Fracture Behaviors of HSLA Steel Weld Joints. Int. J. Fatigue
**2020**, 137, 105644. [Google Scholar] [CrossRef] - Lago, J.; Trško, L.; Jambor, M.; Nový, F.; Bokůvka, O.; Mičian, M.; Pastorek, F. Fatigue Life Improvement of the High Strength Steel Welded Joints by Ultrasonic Impact Peening. Metals
**2019**, 9, 619. [Google Scholar] [CrossRef][Green Version] - Šebestová, H.; Hornik, P.; Mrňa, L.; Jambor, M.; Hornik, V.; Pokorný, P.; Hutař, P.; Ambrož, O.; Doležal, P. Fatigue Properties of Laser and Hybrid Laser-TIG Welds of Thermo-Mechanically Rolled Steels. Mater. Sci. Eng. A
**2020**, 772, 138780. [Google Scholar] [CrossRef] - Moravec, J.; Sobotka, J.; Solfronk, P.; Thakral, R. Heat Input Influence on the Fatigue Life of Welds from Steel S460MC. Metals
**2020**, 10, 1288. [Google Scholar] [CrossRef] - Hong, J.K.; Dong, P.; Brust, F.; Forte, T. Effect of Welding Induced Residual Stresses on the Fatigue Behavior of T-Joints; SAE Technical Paper: Warrendale, PA, USA, 1998. [Google Scholar]
- Webster, G.; Ezeilo, A. Residual Stress Distributions and Their Influence on Fatigue Lifetimes. Int. J. Fatigue
**2001**, 23, 375–383. [Google Scholar] [CrossRef] - James, M.; Hughes, D.; Chen, Z.; Lombard, H.; Hattingh, D.; Asquith, D.; Yates, J.; Webster, P. Residual Stresses and Fatigue Performance. Eng. Fail. Anal.
**2007**, 14, 384–395. [Google Scholar] [CrossRef][Green Version] - Lee, C.-H.; Chang, K.-H. Comparative Study on Girth Weld-Induced Residual Stresses between Austenitic and Duplex Stainless Steel Pipe Welds. Appl. Therm. Eng.
**2014**, 63, 140–150. [Google Scholar] [CrossRef] - Harati, E.; Karlsson, L.; Svensson, L.-E.; Dalaei, K. The Relative Effects of Residual Stresses and Weld Toe Geometry on Fatigue Life of Weldments. Int. J. Fatigue
**2015**, 77, 160–165. [Google Scholar] [CrossRef] - Kang, H.T.; Lee, Y.-L.; Sun, X.J. Effects of Residual Stress and Heat Treatment on Fatigue Strength of Weldments. Mater. Sci. Eng. A
**2008**, 497, 37–43. [Google Scholar] [CrossRef] - Jandera, M.; Machacek, J. Residual Stresses and Strength of Hollow Stainless Steel Sections. 2007, pp. 262–263. Available online: https://www.researchgate.net/profile/Michal-Jandera/publication/268358021_RESIDUAL_STRESSES_AND_STRENGTH_OF_HOLLOW_STAINLESS_STEEL_SECTIONS/links/54b78e070cf2bd04be33a1f3/RESIDUAL-STRESSES-AND-STRENGTH-OF-HOLLOW-STAINLESS-STEEL-SECTIONS.pdf (accessed on 2 November 2022).
- Dakhlaoui, R.; Braham, C.; Baczmański, A. Mechanical Properties of Phases in Austeno-Ferritic Duplex Stainless Steel—Surface Stresses Studied by X-Ray Diffraction. Mater. Sci. Eng. A
**2007**, 444, 6–17. [Google Scholar] [CrossRef] - Johansson, J.; Odén, M. Load Sharing between Austenite and Ferrite in a Duplex Stainless Steel during Cyclic Loading. Metall. Mater. Trans. A
**2000**, 31, 1557–1570. [Google Scholar] [CrossRef] - Jang, D.; Watkins, T.; Kozaczek, K.; Hubbard, C.; Cavin, O. Surface Residual Stresses in Machined Austenitic Stainless Steel. Wear
**1996**, 194, 168–173. [Google Scholar] [CrossRef] - Ragavendran, M.; Vasudevan, M.; Hussain, N. Study of the Microstructure, Mechanical Properties, Residual Stresses, and Distortion in Type 316LN Stainless Steel Medium Thickness Plate Weld Joints. J. Mater. Eng. Perform.
**2022**, 31, 5013–5025. [Google Scholar] [CrossRef] - ČSN EN 10027-1; Systémy Označování Ocelí–Část 1: Stavba Značek Ocelí. Praha: Úřad pro Technickou Normalizaci, Metrologii a Státní Zkušebnictví, 2017; 40 s. Třídící Znak 42 0011.
- ČSN EN 10027-2; Systémy Označování Ocelí–Část 2: Systém Číselného Označování. Praha: Úřad pro Technickou Normalizaci, Metrologii a Státní Zkušebnictví, 2016; 24 s. Třídící Znak 42 0011.
- Moravec, J.; Sobotka, J.; Novakova, I.; Bukovska, S. Assessment the Partial Welding Influences on Fatigue Life of S700MC Steel Fillet Welds. Metals
**2021**, 11, 334. [Google Scholar] [CrossRef]

**Figure 2.**Drawing of the sample for simulations in Gleeble (in mm) [34].

**Figure 3.**Sample drawing for fatigue testing acc. to standard EN 3987 (in mm) [35].

**Figure 9.**Courses of residual stresses after application of temperature cycles, for sample 1 (red curve), for sample 2 (blue curve), for sample 3 (grey curve).

**Figure 10.**Courses of residual stresses after application of temperature cycles (red curve) and after annealing to reduce residual stresses (blue curve).

**Figure 13.**Comparison of all measured S–N curves, base material (black curve), annealed material at 550 °C for 2 h (pink curve), after TC (orange curve), after TC + HT 550 °C for 2 h (blue curve).

C | Si | Mn | P | S | Al | Nb | V | |

ČSN EN 10149-2 | max. 0.12 | max. 0.6 | max. 2.2 | max. 0.025 | max. 0.010 | min. 0.015 | max. 0.09 | max. 0.2 |

Experiment | 0.050 | 0.196 | 1.914 | 0.006 | 0.006 | 0.037 | 0.063 | 0.072 |

Ti | Mo | B | N | Ni | Cr | W | ||

ČSN EN 10149-2 | max. 0.25 | max. - | max. 0.005 | - | - | - | - | |

Experiment | 0.056 | 0.112 | 0 | 0.013 | 0.153 | 0.035 | 0.035 |

Sample No. | YS [MPa] | UTS [MPa] | A_{g} [%] | A_{30} [%] |
---|---|---|---|---|

Basic material | 748 ± 9 | 851 ± 1 | 11.08 ± 0.62 | 24.03 ± 0.62 |

Annealing material (550 °C_2 h) | 745 ± 3 | 785 ± 3 | 9.69 ± 0.12 | 21.16 ± 0.29 |

Basic material | σ_{A} [MPa] | 580 | 550 | 527.5 | 505 | 490 |

Nf [1] | 153,695 | 234,942 | 1,056,376 | 1,804,894 | 1,063,721 | |

σ_{A} [MPa] | 475 | 468 | 461 | 455 | 447.5 | |

Nf [1] | 804,513 | 1,687,452 | 2,420,822 | 7,153,698 | 10^{7} | |

550 °C 2 h | σ_{A} [MPa] | 580 | 565 | 550 | 546 | 542.5 |

Nf [1] | 89,479 | 292,247 | 288,898 | 1,964,321 | 3,083,698 | |

σ_{A} [MPa] | 535 | 535 | 527,5 | 520 | 500 | |

Nf [1] | 589,138 | 1,011,574 | 3,680,777 | 8,881,583 | 10^{7} |

After TC | σ_{A} [MPa] | 520 | 490 | 460 | 400 | 370 |

Nf [1] | 78,412 | 290,364 | 354,888 | 536,242 | 1,138,628 | |

σ_{A} [MPa] | 360 | 350 | 345 | 340 | 335 | |

Nf [1] | 1,968,348 | 5,698,176 | 3,458,265 | 6,483,620 | 10^{7} |

After TC + annealing | σ_{A} [MPa] | 600 | 570 | 540 | 500 | 490 |

Nf [1] | 81,275 | 136,846 | 436,195 | 874,693 | 1,297,314 | |

σ_{A} [MPa] | 480 | 472.5 | 465 | 457.5 | 450 | |

Nf [1] | 2,769,674 | 4,181,239 | 6,583,912 | 8,826,743 | 10^{7} |

Publisher’s Note: MDPI stays neutral with regard to jurisdictional claims in published maps and institutional affiliations. |

© 2022 by the authors. Licensee MDPI, Basel, Switzerland. This article is an open access article distributed under the terms and conditions of the Creative Commons Attribution (CC BY) license (https://creativecommons.org/licenses/by/4.0/).

## Share and Cite

**MDPI and ACS Style**

Bukovská, Š.; Moravec, J.; Solfronk, P.; Pekárek, M. Assessment of the Effect of Residual Stresses Arising in the HAZ of Welds on the Fatigue Life of S700MC Steel. *Metals* **2022**, *12*, 1890.
https://doi.org/10.3390/met12111890

**AMA Style**

Bukovská Š, Moravec J, Solfronk P, Pekárek M. Assessment of the Effect of Residual Stresses Arising in the HAZ of Welds on the Fatigue Life of S700MC Steel. *Metals*. 2022; 12(11):1890.
https://doi.org/10.3390/met12111890

**Chicago/Turabian Style**

Bukovská, Šárka, Jaromír Moravec, Pavel Solfronk, and Milan Pekárek. 2022. "Assessment of the Effect of Residual Stresses Arising in the HAZ of Welds on the Fatigue Life of S700MC Steel" *Metals* 12, no. 11: 1890.
https://doi.org/10.3390/met12111890